Research Article  Open Access
Ali Raza, Qaiser uz Zaman Khan, Afaq Ahmad, "Numerical Investigation of LoadCarrying Capacity of GFRPReinforced Rectangular Concrete Members Using CDP Model in ABAQUS", Advances in Civil Engineering, vol. 2019, Article ID 1745341, 21 pages, 2019. https://doi.org/10.1155/2019/1745341
Numerical Investigation of LoadCarrying Capacity of GFRPReinforced Rectangular Concrete Members Using CDP Model in ABAQUS
Abstract
The present work demonstrates the nonlinear finite element analysis (NLFEA) of 13 concentrically and eccentrically loaded short rectangular concrete column specimens reinforced with GFRP and conventional steel bars. GFRP bars are lightweight having the high tensile strength and high corrosion resistance. An NLFEA model for the rectangular concrete specimens was developed using the commercial software ABAQUS Standard and calibrated for different materials and geometric parameters based on the previous experimental test results of the studied specimen. The behavior of reinforced concrete was modelled using the concrete damaged plasticity (CDP) model, the behavior of steel bars was simulated as a bilinear elastoplastic material, and the GFRP bars were considered as a linear elastic material. After the calibration of CDP parameters, the control sample was used for the further numerical parametric analysis to investigate the effect of critical parameters, i.e., the area of concrete (A_{c}), the compressive strength of concrete (), and the ratio of longitudinal reinforcement () and transverse reinforcement () on the loadcarrying capacity of columns. The results show that the selected NLFEA model can simulate the behavior of columns accurately and there was good agreement of numerical results obtained from ABAQUS Standard with the experimental results.
1. Introduction
Glass fiberreinforced polymer (GFRP) is a lightweight, corrosion resistant, nonmagnetic and electrically insulating material with a very high tensile strength and low thermal conductivity. GFRP bars are used as a viable replacement of steel bars in reinforced concrete structures. Due to nonmagnetic and nonconductive properties of the GFRP material, it can be preferred to use near sensitive instruments in laboratories and hospitals [1–4]. Also, the smaller concrete cover is used for GFRPreinforced members due to the corrosionresistant property of GFRP bars. In the wastewater and chemical treatment plants, marine structures, and the structures exposed to deicing salts, the corrosion of conventional steel causes the reduction of the serviceability of structures. Due to this problem, the steelreinforced concrete (RC) structures in such aggressive environments have about 50 years of life only. The replacement of steel with FRP composites such as GFRP bars could be useful in saving the tremendous repair costs for longterm serviceability and durability of structures [5]. Throughout the life of RC structures, GFRP bars have been found to be economical. Fiberreinforced polymers (FRP) bars having a density of less than onequarter of that of steel bars with higher tensile strength and corrosion resistance in chemical environments offer a number of advantages over steel [6, 7]. Furthermore, due to high strength, high corrosion resistance, and less concrete cover, GFRP bars have high utilization for the retrofitting purpose of old or damagereinforced concrete building [8].
Extensive experimental work has been done as compared to the numerical work by research groups on the behavior of GFRP RC compression and flexural members. Nguyen et al. [9] studied lateraltorsional buckling (LTB) of fiberreinforced polymer (FRP) Ibeams by using nonlinear finite element analysis and concluded that due to change in load height and end warping fixity, the beam with FRP has larger effect on buckling strength as compared to the beam with steel elastic constants. Yang et al. [10] examined the damage behavior of GFRP RC beams by performing the experimental and FEA and reported that the developed FEA model is accurate enough to predict the damage behavior of GFRP RC beams. Amiri et al. [11] presented a FE model of reinforced geopolymer concrete flexural members using commercial software ABAQUS and found a deviation in experimental and numerical results for deflections, but the crack pattern showed good agreement. Najafgholipour et al. [12] conducted the FEA of reinforced concrete exterior and interior beamcolumn joints by using the CDP model in ABAQUS and studied deformations, joint shear capacity, and cracks patterns with the conclusion that FEA results are in good agreement with the experimental results. Prachasaree et al. [5] studied the behavior of GFRP RC columns with different types of stirrups and concluded that the effect of longitudinal GFRP reinforcement on the strength of a column is slight, but transverse reinforcement significantly affects the confining pressure by increasing the concrete strength and inelastic deformation. Alsayed et al. [13] performed the tests on 450 × 250 × 1200 mm columns under concentric loading and concluded that, by using same longitudinal reinforcement ratio of steel and GFRP bars, the capacity of GFRPreinforced columns is decreased by 13%. Nunes et al. [14] conducted the experimental and numerical investigations on GFRP pultruded columns which were subjected to eccentric loadings and concluded that when the load is applied within the kern boundary, the loadcarrying capacity of the column is decreased up to 40%. Furthermore, a good agreement was achieved between experimental and numerical results. Turvey and Zhang [15] also conducted an experimental and numerical study to investigate the failure mechanism of postbuckled GFRPreinforced short concrete columns. The numerical study was conducted by using both generalized beam theory (GBT) and ABAQUS.
From the literature review, it has been observed that the numerical behavior of the GFRPreinforced compression members using FEA software ABAQUS is less defined and no numerical parametric study was conducted. Therefore, to accurately simulate and analyze the numerical behavior of GFRP reinforcement in columns and to provide new design codes for GFRP reinforcement, an experimental and numerical parametric study is needed by examining the critical parameters that influence the axial capacity of RC columns. The primary objective of the present research is to propose a NLFEA model in ABAQUS which accurately simulates the behavior of reinforced concrete and to validate it against the previous experimental test results of loaddeflection curves of 13 column specimens. After the validation of the NLFEA model, this calibrated numerical model was used to establish the loaddeflection curves of columns compared with previous experimental results from Elchalakani and Ma [16], and then a numerical parametric study of steel and GFRP control specimens was done. The crack patterns of concrete in RC columns were also studied. Finally, the experimental and FEA results of concentrically loaded steel and GFRP RC columns were compared with theoretical results. The significance of the present work is that the proposed FEA ABAQUS model can be utilized for the further analysis of different parameters of columns.
2. Finite Element Modelling
2.1. General Methodology
Numerical simulations of GFRPreinforced concrete columns were done by using commercial software ABAQUS Standard 6.12. During the modelling of specimens, the concrete material models, boundary conditions, and different geometric and material parameters were discussed in detail. The concrete material was modelled as a homogeneous 3D solid section. Drucker–Prager plasticity model was used for the numerical simulations of FRP confined concrete [17–19]. Generally, the numerical model should be rich enough to be capable of capturing the critical and essential phenomena but should not be complex enough to increase the analysis time of the computer. After simulating the geometry of the control model, it was calibrated for dilation angle, stress ratio, shape factor, plastic potential eccentricity, and viscosity parameter of the concrete damaged plasticity (CDP) model, different element types, and mesh sizes to achieve better results as compared with previous experimental results.
2.2. Model Geometry, Boundary Conditions, and Loading
All the steel and GFRP RC columns were fixed at the bottom, and the top end was kept free in all directions with the applied axial loading. Embedded region constraint available in ABAQUS Standard was used to define the bonding of reinforcing bars, i.e., steel and GFRP bars, with concrete which limits the nodes of reinforcing bars elements to the compatible degrees of freedom (DOF) of the host region elements (concrete), as shown in Figure 1(c). To determine the axial loaddeflection history of reinforced concrete columns up to failure, a static monotonic loading was applied on the top by the displacement control technique. An induced displacement of 20 mm was applied on the top center of concentric columns and at a distance equal to required eccentricity from the center of specimens along the weaker axis of eccentric columns. Steel plates of 50 mm thickness were attached to the top and bottom of the columns using “tie constraint” for the application of boundary conditions and equal distribution of applied loads. These plates were considered as rigid elements with Young’s modulus of 210 GPa and density of 7.85·10^{−9} ton/mm^{3}. The geometry and the modelling details of the finite element models of steelreinforced columns are shown in Figure 1.
The different concrete material properties and loading increments and sizes in Step Module of ABAQUS Standard are given in Table 1. The modulus of elasticity (E_{c}) of concrete was calculated using the ACI code given by

The master and slave surface concept was used to define the interaction between concrete columns and steel plates. The bottom surface of the top steel plate and the bottom surface of the column were taken as master surfaces, and the top surface of the column and the top surface of the bottom steel plate were considered as slave surfaces. In other words, the load transferring surfaces were taken as master surfaces. The smaller concrete clear cover was used for GFRP RC specimens due to the corrosion resistant property of GFRP bars according to Elchalakani et al. The geometry and modelling details of finite element models of GFRP RC columns were shown in Figure 2.
A total of 13 fullscale rectangular RC column specimens were modelled in ABAQUS under different loading conditions, from which 6 specimens were reinforced longitudinally and transversely with steel bars and remaining 7 specimens were reinforced with GFRP bars. Three loading eccentricities (25 mm, 35 mm, and 45 mm) and three ligature spacings (75 mm, 150 mm and 250 mm) were used to study their effect on the loaddeflection behavior of compression members.
The used ultimate compressive strength of concrete was 32 MPa. The geometric and material characteristics of all specimens are shown in Table 2.

2.3. Concrete Damaged Plasticity (CDP) Model
In ABAQUS, there are three constitutive models for defining the inelastic behavior of concrete including concrete smeared cracking model (CSCM), concrete damaged plasticity (CDP) model, and brittle cracking concrete (BCC) model. The CDP model deals with plastic behavior, compressive behavior, tensile behavior, confinement, and damage mechanism of concrete and has the potential to converge the results to accuracy as compared with other models. In comparison with steel, concrete exhibits nonlinearity from the start when subjected to tension or the compression test.
The CDP model defines two failure mechanisms of concrete which are compressive crushing and tensile cracking. The CDP model is commonly accepted for the modelling of the nonlinear behavior of reinforced concrete [20–22]. Thus, in the current study, the behavior of the concrete material was defined by using the CDP model given by Liu and Chen [23], as shown in Figure 3 which describes the relationship between inelastic strain, plastic strain, and compression stress and strain of concrete. The damage parameter d_{c}, plastic strain ɛ^{pl}, and inelastic strain ɛ^{in} are determined using [23]. The CDP model in ABAQUS consists of plastic behavior, compressive behavior, and tensile behavior of concrete.
2.3.1. Plastic Behavior of Concrete
The parameters required to define the plasticity model of concrete are dilation angle , the plastic potential eccentricity of concrete (ɛ), the ratio of compressive stress in the biaxial state to the compressive stress in the uniaxial state , the shape factor of the yielding surface in the deviatoric plane (K_{c}), and viscosity parameter. The values of all these parameters were obtained from calibration. The CDP model recommended values of the yield shape surface, K_{c}, and eccentricity, ɛ, which are 2/3 and 0.1, respectively. The specified value of , by ABAQUS user manual [24], is 1.16. Also to quantify this stress ratio, Papanikolaou and Kappos [25] proposed equation (2) based on a large statistical data:
2.3.2. Compressive Behavior of Concrete
To define the compressive behavior of concrete in the CDP model, it is essential to give inelastic strain ε^{in} in further increased degree so that compression failure of concrete can be defined at increased strain and peak elastic stress of concrete is to be provided in the compression behavior. According to Eurocode 2, the compressive stressstrain diagram for concrete has been shown in Figure 4. The linear elastic behavior can be taken up to 0.4f_{cm} according to Kmiecik and Kamiński [26]. To determine the strain ε_{c1} at the average compressive strength of concrete and ultimate strain ε_{cu1}, Majewski [27] proposed the approximate relationships based on the experimental results given by the following equation:
Equation (4) given by Eurocode [28] for nonlinear behavior of structures was used in this research for modelling the stressstrain relationship of concrete:where
Desayi and Krishnan [29] also proposed the equation for the stressstrain relationship of nonlinear behavior of structures given by the following equation which can also be used:where is the compressive strain at peak loads and is equal to 0.002 according to Mander et al. [30].
2.3.3. Tensile Behavior of Concrete
For the simulation of tensile behavior of concrete, a stressstrain relationship at the postfailure condition is used for accounting tension stiffening, the interaction of reinforcement with concrete and strain softening. The tension stiffening model given by Nayal and Rasheed [31] is applicable for both fiberreinforced polymer (FRP) and steelreinforced concrete. Wahalathantri et al. [32] modified the tension stiffening model of reinforced concrete given by Nayal and Rasheed [31] which was used for the present study and is shown in Figure 5. In this modified model, the only change was that the sudden drop of the tensile stressstrain curve at a critical strain was from ultimate stress to 0.77 in place of 0.80.
The concrete ultimate tensile strength was estimated by using the following equation proposed by Wang et al. [33] and Genikomsou and Polak [34]:
2.4. Modelling of Reinforcing Bars
An isotropic linear elastic behavior was assumed to model the GFRP bars in ABAQUS, up to failure without applying any damage criterion [35, 36]. The linear elastic behavior of GFRP reinforcing bars was assumed because of the reason that they show brittle failure after yielding without going to the plastic range as shown in Figure 6.
The nonlinear behavior of steel bars was simulated as a bilinear elastoplastic material using a strain hardening ratio of 0.01, as recommended by Kachlakev and Miller [37]. The bilinear stressstrain model for the longitudinal steel bars is shown in Figure 7.
Twonoded deformable truss elements having three DOF (translations in X, Y, and Z global coordinate directions) at each node (T3D2R) were utilized for the simulations of all reinforcing bars. Only four parameters were needed for modelling of reinforcing bars which are Poisson’s ratio () and modulus of elasticity for elastic behavior and yield strength and corresponding plastic strain for plastic behavior of steel bars. In this study, Poisson’s ratio () was assumed as 0.3 for steel bars and 0.25 for GFRP bars [35]. The physical properties of GFRP and steel bars used in this research are given in Tables 3 and 4, respectively.


2.5. Calibration and Convergence of Model
For the convergence and validation of the finite element model and to investigate the role of various geometric and material parameters to produce accurate results, the effect of varying the mesh size, element types, dilation angle, shape factor, eccentricity, stress ratio, and viscosity parameter was studied. This calibration process was done based on the test results of control specimen S45150. The calibrated FE model was then used to conduct the numerical analysis of all remaining column specimens.
The effect of the viscosity parameter on the loaddeflection response of columns is shown in Figure 8. The value of the viscosity parameter is influenced by time increment size. To achieve the best results, small values of the viscosity parameter should be used as compared with the pseudotime of finite element analysis and it should be taken near about to 15% of the time increment step to get the improved results as proposed by Lee and Fenves [38].
The time increment step was kept automatic, and initial and maximum increment sizes were kept as 0.01 throughout the analysis. The best approximate was achieved by using a value of 0.0058 for the viscosity parameter while keeping the dilation angle and mesh size of 35° and 20 mm, respectively.
For concrete, the dilation angle is a material parameter and physically, and it is interpreted as an internal friction angle of concrete. A sensitivity analysis for the dilation angle was performed to check out the parameter influence on the axial loaddeflection curve of the control sample. Drucker–Prager plastic potential function is defined by the following equation:where is the dilatancy parameter for concrete. The flow potential function represented by equation (9) is used by the CDP model which is Drucker–Prager hyperbolic function derived from equation (8):where is the dilation angle, is the eccentricity of the plastic flow potential function required to adjust the shape of hyperbola, and is the uniaxial tensile strength of concrete at failure. By using Drucker–Prager plastic potential function (equation (8)), equation (9) can be rewritten as
For = 0.2 as defined by Lee and Fenves [39], the value of the dilation angle is 31°. Voyiadjis and Taqieddin [40] and Wu et al. [41] proposed that the value of dilatancy parameter ranges between 0.2 and 0.3. For this range of , the dilation angle () should be between 31° and 42°. In the present study, the dilation angle values between 30° and 45° were examined giving accurate results to previous experimental data at 35° when the viscosity parameter was 0.0058 and mesh size was 20 mm. So, dilation angle of 35° was used for the finite element (FE) simulations of all specimens.
Figure 9 shows the effect of the dilation angle on the axial loadaxial deformation curve for the control specimen (S45150). It can be noted from the loaddeflection curve that the influence of the variation of dilation angle on results is relatively small as compared with the effect of the viscosity parameter.
The effect of variation of the shape factor (K_{c}) on the loaddeflection behavior of the control specimen was shown in Figure 10. It was observed that, by increasing the value of K_{c}, the peak of the loaddeflection curve moves downwards giving more error. Thus, K_{c} with a value of 0.667 is best suited for the plastic behavior of concrete which is also recommended by the CDP model.
The effect of the plastic potential eccentricity was also checked on the loaddeflection behavior of the control specimen. It was observed that the effect of variation of eccentricity on the loaddeflection behavior of columns is negligible, as shown in Figure 11. Thus, the default value of this parameter was selected in the present study. The calibration for the stress ratio was done giving the negligible effect of variation, and hence, a default value of 1.16 was selected as recommended by the ABAQUS user manual 6.10. The effect of the variation of the stress ratio was presented in Figure 12.
The convergence due to the mesh size and mesh type was also studied. The numerical model is mesh size dependent due to the strain localization which occurs within a few elements leaving the remaining elements to be unloaded. Due to use of finer mesh size, the formation of narrow bands of localization occurs and numerical convergence of the equations fails [34]. With coarse mesh sizes, the obtained results showed a significant divergence from experimental results which was not accepted. To converge these results, close to experimental results, finer mesh sizes were used. Furthermore, an even finer mesh size gave the results which were approximately the same as given by the previous mesh size used, but the time of analysis was increased for computations.
In Figure 13, the numerical results of the loaddeflection curve for the control specimen are presented with 60 mm, 50 mm, 40 mm, 30 mm, 25 mm, 20 mm, and 15 mm mesh sizes. Figure 13 depicts that the mesh size of 20 mm is finer enough to achieve accurate results. Small time increments were used in the study to overcome the convergence difficulties during nonlinear analysis and to make sure that the analysis will be done according to the loaddeflection curve.
The convergence of the FEA model due to element types of concrete and reinforcing bars is shown in Figure 14. The calibration of the concrete material was done for standard 3D stress linear and quadratic hexahedral elements with reduced integration (C3D8R and C3D20R), triangular prism elements with hybrid formulation (C3D6H and C3D15H), and linear and quadratic tetrahedral elements with hybrid formulation (C3D4H and C3D10H), and the calibration of reinforcing bars was done using standard 3D truss elements with reduced integration (T3D2R and T3D3R) and beam elements with hybrid formulation (B31H and B32H). The analysis time was captured to be less for C3D8R and T3D2R elements with relatively accurate results. Furthermore, the previous research [12, 42, 43] has shown that C3D8R elements follow constitutive law of integration accurately and usually it is the most suitable element type for the nonlinear analysis of structures. Generally, hexahedral truss elements have preference over beam elements because of their simple geometry with accurate results and less time of analysis. Furthermore, the nodes of hexahedral elements of the concrete material are kinematically constrained to hexahedral truss elements of reinforcing bars in the embedded region constraint of ABAQUS. Therefore, the average displacements of nodes of concrete hexahedral elements and truss hexahedral elements of bars will be equal and give accurate results, and thus, these element types were used in this study giving the accuracy. It was noted that the effect of variation of 3D linear stress elements of the concrete and 3D truss elements of the reinforcement on the loaddeflection curve was very less, but quadratic elements of concrete and beam elements of reinforcing bars presented some discrepancy from experimental results.
(a)
(b)
(c)
(d)
The concrete damaged plasticity model parameters, such as the dilation angle, flow potential eccentricity, the ratio of biaxial to uniaxial compressive stresses, viscosity parameter, and shape factor for yielding surface of concrete, are taken according to Table 5.

3. Discussion of Finite Element Analysis Results
The testing positions and boundary conditions of concentric and eccentric column specimens are shown in Figure 15 with 0 mm, 25 mm, and 45 mm eccentricities, respectively. The detailed summary of the experimental test results of 13 rectangular concrete columns from Elchalakani and Ma [16] and finite element analysis (FEA) results from the current study are presented in Figure 16 in terms of ultimate loads and axial deflection at ultimate loads.
(a)
(b)
3.1. Control Specimen (S45150)
The final axial loaddeformation results for control specimen S45150 are represented by Figure 17 after the calibration for different materials and geometric parameters. It showed that the experimental results of ultimate loads and deformations were traced precisely by the FEA model. The discrepancies for the control specimen were 1.58% and 14% for ultimate load and corresponding deflection, respectively.
3.2. Ultimate Load and Axial Deflection at Ultimate Load
The finite element model, calibrated for different parameters, was applied to analyze the remaining compression members. Most of the columns were traced accurately up to peak loads. The finite element models of steelreinforced columns achieved an average difference of 3.86% in ultimate load and 15.20% in axial deflection at ultimate load and that of GFRPreinforced columns achieved an average difference of 3.78% in ultimate load and 18.54% in corresponding axial deflection at ultimate load as compared with experimental results. However, the finite element models of concentrically loaded columns (SC75, SC150, GC75, GC150, and GC250) had a tendency of overestimation of the ultimate loads and deflections at ultimate loads. From eccentrically loaded columns, the overestimation of ultimate load only occurred for G25150. The most significant discrepancy in the finite element simulations of columns was observed for S3575 with 13.57% difference in ultimate load and for SC75 with 27.07% difference in axial deflection at ultimate load from experimental results.
3.3. LoadDeflection Behavior of SteelReinforced Columns
3.3.1. Concentrically Loaded Columns
Figure 18 shows the experimental and finite element analysis results of loaddeflection curves for concentric steelreinforced rectangular concrete columns with stirrups spacings of 150 mm and 75 mm.
It is clear from Figure 18 that FEA results of steel RC concentric columns were in close agreement with experimental results up to peak behavior. After peak loading, FEA results were a little bit larger than experimental results. This may occur because of the assumption of a perfect bond between the reinforcing bars and concrete. The concentric column specimen SC75 showed a difference of 1.79% in ultimate load and 27.07% in the corresponding deflection as compared with experimental results. On the contrary, SC150 showed a difference of 0.56% and 21.28% in ultimate load and axial deflection at ultimate load, respectively.
3.3.2. Eccentrically Loaded Columns
The axial loadaxial deflection curves for eccentric steelreinforced rectangular concrete columns with ligature spacings of 150 mm and 75 mm and test eccentricities of 25 mm, 35 mm, and 45 mm are shown in Figure 19. The FEA results of eccentric columns were in high accuracy with experimental test results in the elastic range. The ultimate loads given by FEA simulations were a little bit less than the experimental results for all the eccentric loaded steelreinforced columns.
(a)
(b)
(c)
(d)
The finite element simulations produced results such that the differences of 0.31% and 13.57% were observed for ultimate loads and the differences of 17.48% and 2.40% were observed for axial deflections at ultimate loads for specimens S2575 and S3575, respectively. The numerical simulations of columns with 150 mm ligature spacing (S25150 and S45150) gave discrepancy of 5.34% and 1.58% for ultimate loads and 8.94% and 14.06% for corresponding axial deflection at ultimate load, respectively. The behavior of eccentric columns was traced better as compared with concentric columns.
3.3.3. Ultimate Load against Eccentricity
Figure 20 represents the ultimate loads of steelreinforced columns as a function of the test eccentricity level. It represents that the ultimate load decreases as the test eccentricity of columns increases. The decrease in ultimate load with an increase of eccentricity is somewhat larger for FEA results. When eccentricity level increases, the longitudinal compressive stresses increase on that side of columns causing the buckling of columns and, consequently, columns fail at lower loads. From Figure 20, one can observe that when FEA load is applied with an eccentricity equal to 25 mm, there is a reduction of ultimate load up to roughly 700 kN and when FEA load is applied with an eccentricity equivalent to 45 mm, there is an ultimate load reduction of roughly 900 kN.
So, it can be monitored that a loss of 43.86% and 64.26% in ultimate load occurs for 25 mm and 45 mm eccentricities, respectively, when compared to an identical concentrically loaded column. Moreover, for small eccentricities within the crosssectional kern, the reduction in ultimate load occurs with a linear trend approximately.
3.4. LoadDeflection Behavior of GFRPReinforced Columns
3.4.1. Concentrically Loaded Columns
Figure 21 represents the experimental and finite element analysis (FEA) results of loaddeformation curves for GFRPreinforced concentric concrete columns with stirrups spacings of 250 mm, 150 mm, and 75 mm. The finite element analysis (FEA) results of GFRP concentric columns were in good agreement with experimental behavior up to ultimate loads. After ultimate loading, FEA results were larger than experimental results with respect to both ultimate loads and deformations at ultimate loads similar to steel columns. These increased numerical results may be due to the fact that a perfect tie bond between concrete and GFRP reinforcing bars was assumed.
The concentric column specimen GC75 showed the difference of 2.57% in ultimate load and 25.35% in the corresponding deflection as compared with experimental results. The specimen GC150 showed discrepancy of 1.27% and 17.47% in ultimate load and axial deflection at ultimate load, respectively. The column with ligature spacing of 250 mm gave the differences of 1.79% in ultimate load and 21.07% in axial deflection at ultimate load. The FEA response of GC150 was slightly stiffer than the experimental test results.
3.4.2. Eccentrically Loaded Columns
The FEA results of GFRPreinforced eccentric columns were in high accuracy with experimental results up to peak behavior. The graphical representations of axial load against the axial deflection for eccentrically loaded GFRPreinforced columns with tie spacings of 75 mm and 150 mm and eccentricities of 25 mm, 35 mm, and 45 mm are shown in Figure 22. The ultimate loads shown by FEA simulations were a little bit less than the experimental results for all the eccentric columns except G25150.
(a)
(b)
(c)
(d)
The finite element simulations produced results such that the difference of 2.34% was observed for ultimate load and a difference of 21.37% was observed for axial deflection at ultimate load for the specimen G2575 as compared with experimental test results. G3575 showed the differences of 11.84% and 17.46% for ultimate load and corresponding deflection. The numerical simulations of columns with a transverse reinforcement spacing of 150 mm (G25150 and G45150) gave discrepancy of only 0.42% and 6.23% for ultimate loads and 10.29% and 16.75% for axial deflection at ultimate load, respectively. The finite element simulations in ABAQUS Standard terminated at the points where sufficient deformation occurred in an element of the specimen. Therefore, a finer mesh is the most suitable for analysis. However, the FE simulations of ultimate load and deformation at ultimate load were conducted at a high accuracy.
3.4.3. Ultimate Load against Eccentricity
Figure 23 represents the ultimate loads of GFRPreinforced columns as a function of testing eccentricity. It clarifies that the ultimate load is inversely proportional to the test eccentricity of columns. Due to an increase of eccentricity, the stresses increase on the either side of the column, allowing the column to buckle on that side by decreasing the axial capacity. When test eccentricity is equivalent to 25 mm, the FEA ultimate load reduces up to roughly 600 kN and when the load is applied with an eccentricity of 45 mm, the reduction in FEA ultimate load is roughly 950 kN. So, it can be observed that a loss of 39.74% in ultimate load occurs for 25 mm eccentricity and 60.42% loss occurs for 45 mm eccentricity when compared to an identically loaded column. These results show that the geometry of GFRPreinforced beamcolumn connections in RC structures should be adequately simulated because a small eccentricity may cause a large reduction in ultimate loads. Moreover, it is clear from Figure 23 that the ultimate load decreases linearly as the eccentricity of columns increases. The decrease in ultimate load with an increase of the eccentricity is larger for numerical results as compared with the experimental test results.
4. Numerical Parametric Study
To study the influence of different variables on the loaddeflection behavior of the steel and GFRP RC columns (S45150 & G45150), each of the following variables was studied: (1) compressive strength of concrete (); (2) longitudinal reinforcement ratio (); (3) concrete cover (cc); and (4) crosssectional shape of columns.
4.1. Effect of Compressive Strength of Concrete ()
To investigate the effect of varying the compressive strength of concrete on axial load and axial deflection response of control specimens, of 10 MPa, 20 MPa, 30 MPa, 40 MPa, and 50 MPa was considered as represented in Figure 24. The compressive and tensile behavior of concrete in the CDP model was changed according to the compressive strength, but the parameters of plastic behavior were kept the same as calibrated. It was observed that the maximum ultimate capacity of the steel RC column (S45150) increased up to 145% and that of the GFRP RC column (G45150) increased up to 193.6% at constant longitudinal reinforcement ratio () of 1.13% when of concrete increased from 10 MPa to 50 MPa. GFRP RC columns showed on average 16% less axial loadcarrying capacity as compared with their steelreinforced concrete counterparts at 1.13% reinforcement ratio. The maximum increase in axial deflection at the ultimate axial load was 57% and 60% at of 1.13% by increasing the concrete strength from 10 MPa to 50 MPa for steel and GFRP RC column, respectively. The loaddeflection curves showed a higher initial stiffness as of concrete increased.
(a)
(b)
Similarly, it was observed that the maximum ultimate capacity of the steel control specimen increased up to 193% and that of the GFRP RC column increased up to 215% at the constant concrete clear cover of 55 mm when of concrete increased from 10 MPa to 50 MPa. GFRP RC columns showed on average 6% less axial loadcarrying capacity as compared with their steelreinforced concrete counterparts at 55 mm concrete cover. The maximum increase in axial deflection at ultimate load was 64% at 25 mm concrete cover and 75% at 55 mm cover when concrete strength was increased from 10 to 50 MPa for steel and GFRP RC column, respectively. The results indicated that as the concrete strength increased, the axial loading capacity of columns increased significantly.
4.2. Effect of Longitudinal Reinforcement Ratio ()
The 3D plots of Figure 24 show the effect of different main reinforcements on the load and deflection behavior of steel and GFRP RC columns. Both columns (S45150 and G45150) had a constant transverse reinforcement of 6 mm diameter ties at 150 mm spacing with varying longitudinal reinforcement ratios of 1.13%, 1.63%, 2.90%, 4.09%, and 5.48%. The percentage increase in axial capacity was 110% and 62% at the constant concrete of 10 MPa when ratio was increased from 1.13% to 5.48% for steel and GFRP RC specimen, respectively. When was increased from 1.13% to 5.48%, the maximum increase of 45% and 40% in axial deflection at ultimate load occurred at 10 MPa concrete strength for steel and GFRP RC column, respectively.
Similarly, for both types of RC specimens, a percentage increase of 110% and 60% occurred for the ultimate load at 15 mm cover of concrete by increasing from 1.13% to 5.48%, respectively. GFRP RC columns presented on average 54% and 55% less axial capacity as compared with steel RC columns at 10 MPa concrete strength and 15 mm concrete cover, respectively. The FEA results indicated that both the specimens confirmed the increase in ultimate loadcarrying capacity of columns with the increase of ratio. The steel RC specimen showed more increase in axial capacity by increase of main reinforcement as compared with the GFRP RC specimen.
4.3. Effect of Concrete Cover (cc)
The specimens S45150 and G45150 were modelled with the same transverse reinforcement of 6 mm diameter ties at a spacing to 150 mm with different concrete covers of 15 mm, 25 mm, 35 mm, 45 mm, and 55 mm. It was observed that the ultimate load and axial deflection at ultimate load decreased up to 40% at of 5.48% and 10% at of 1.13% for the steel RC column and 37% at of 5.48% and 27% at of 2.90% for the GFRP RC column, respectively, when the clear concrete cover was increased from 15 mm to 55 mm as presented in Figure 24. GFRPreinforced columns showed on average 76% less axial ultimate load as compared with their steel RC counterparts at 5.48% reinforcing ratio. By increasing the concrete cover, the core area of concrete decreased by providing the less bearing crosssectional area, due to which axial capacity of the steel RC column decreased from 1005 kN to 607 kN, and that of the GFRP RC column decreased from 580 kN to 362 kN when concrete cover increased from 15 mm to 55 mm at of 5.48%.
The decrement of 26% and 13% occurred at 10 MPa by increasing the concrete cover (cc) from 15 mm to 55 mm for steel and GFRP column, respectively. Thus, there should be a suitable concrete cover not to decrease the capacity of the column significantly and to provide sufficient resistance to corrosion of steel. Smaller concrete cover for GFRP RC columns is recommended due to corrosion resistant property of GFRP bars.
4.4. Effect of CrossSectional Shape
Three crosssectional shapes of columns (rectangular, square, and circular) were considered with the same crosssectional area of 41600 mm^{2}, same concrete compressive strength of 32 MPa, the same reinforcements, and the same test eccentricity, as shown in Figure 25. The dimensions of rectangular, square, and circular columns modelled in ABAQUS Standard were 160 × 260 × 1200 mm, 204 × 204 × 1200 mm, and 230 × 1200 mm, respectively.
It can be observed from Figure 26 that squareshaped columns were failed at relatively larger axial loads and larger axial deflections for both steel and GFRP reinforcements. The axial capacities of steel RC square and circular columns were 1.62 and 1.54 times the axial capacity of the steel RC rectangular column. Similarly, the axial peak capacities of GFRP RC square and circular columns were 1.92 and 1.81 times the axial capacity of GFRP RC rectangular column. Therefore, it is concluded that, having the same crosssectional area with the same reinforcement ratios, the square column shows significant ultimate capacity for both steel and GFRPreinforced concrete members. Moreover, the manufacturing of circular GFRP ties is more complex, and they are inappropriate to be used in composite sections such as Ishaped and Tshaped sections.
(a)
(b)
(c)
(d)
5. FEA Cracking Patterns
According to concrete damaged plasticity (CDP) model, the cracking of concrete starts due to positive maximum principal plastic strain (PE). The direction of cracks in reinforced concrete is taken to be normal to maximum positive principal PE, and therefore, the crack patterns are visualized through max. principal PE [34]. For the presentation of cracking patterns, tensile principal stress can be used in ABAQUS, but the plastic principal strains give better visualization of cracks. Figure 27 shows the maximum cracking patterns of steel and GFRP RC columns obtained from FEA simulations in ABAQUS Standard. In all concentric columns, the significant cracks occurred in upper half portion with the rupture of ligatures and concrete core crushing, while in eccentric columns, the tension cracks on the tension side were generated in lower half near the fixed support of columns. The FEA cracking patterns were found to be in good correspondence with experimental cracks. The rigid steel plates tied on top and bottom surfaces of columns were without cracks.
6. Ultimate Strength and Empirical Equations
The theoretical ultimate axial capacity of a short RC column is equal to the summation of the ultimate strength of the concrete material and yielding strength of longitudinal steel bars. In this article, the longitudinal reinforcement was taken the same as in the experimental and FEA work for concentric columns. The concrete cover (cc) was also taken the same as that was in experimental and FEA work, i.e., 40 mm for steel and 20 mm for GFRP RC columns. The gross crosssectional area of GFRP RC columns is more due to less concrete cover (cc). According to the ACI code, the nominal strength (P_{o}) for an axially loaded steelreinforced short column is given by the following equation:where 0.85 is the reduction factor given in ACI 31811 defined as the ratio of inplace strength to cylinder strength of concrete, is the compressive strength of concrete, is the gross crosssectional area of concrete, is the area of longitudinal steel, and is the yield strength of longitudinal steel. ACI 31811 ignores the participation of GFRP bars in axial loadcarrying capacity of columns. The ACI 31811 equation of axial capacity of GFRP RC columns using a reduction factor of 0.85 is shown as follows:where is the crosssectional area of the longitudinal GFRP bars. Currently, Canadian Standard Association (CAN/CSA S80612) allows the use of GFRP bars as main reinforcement in concentrically loaded columns only, neglecting their participation in axial capacity. The recommendation of CSA S80612 is presented in the following equation:where . Afifi et al. [44] presented the following equation by considering the contribution of GFRP bars with a reduction factor :where is the crosssectional area of main GFRP reinforcement, is the tensile strength of GFRP bars, and is the reduction factor for the compressive strength of GFRP bars. Kobayashi and Fujisaki [45] and Tobbi et al. [46] presented a value of 0.35 for this reduction factor.
The charts of Figure 28 show the comparison of experimental, FEA, and theoretical results of concentric steel and GFRP RC columns. It was noticed that the average percentage difference of theoretical peak loads of steel RC concentric columns given by equation (11) from experimental and numerical results was 7.87% and 8.45%, respectively. The results of equations (12) and (13) underestimated the average axial capacity of GFRP RC columns by 20.94% and 22.38%, respectively. However, the average percentage discrepancy of the results of equation (14) from experimental results was only 2.65%. As compared with FEA results, equations (12)–(14) underestimated the peak loads of GFRPreinforced columns on average by 22.38%, 25.30%, and, 2.44%, respectively. Therefore, it was concluded that the design equation provided by Afifi et al. [44] gave the acceptable results of GFRP RC specimens.
(a)
(b)
(c)
(d)
(e)
7. Conclusions
This research paper has endeavored to present the implementation of FEA using ABAQUS to predict the behavior of 13 steel and GFRPreinforced rectangular concentric and eccentric concrete columns subjected to axial loading. The constitutive selected numerical model was first calibrated and validated using test results of control specimen S45150 and was then implemented for the analysis of remaining columns specimens and parametric analysis of two control samples. A theoretical comparative study for concentric steel and GFRP RC columns was also done. The concrete damaged plasticity model was used for the modelling of nonlinearity of reinforced concrete. In finite element modelling, the most challenging aspect is to model the materials accurately, especially the numerical modelling of concrete in concrete structures.
Based on the FEA results documented in the current study in comparison with the experimental results from Elchalakani and Ma [16], the following main conclusions were drawn:(1)From FEA results, it was noted that the average ultimate capacity of GFRPreinforced rectangular concrete columns was 96.14% of the average ultimate capacity of their steelreinforced counterparts. The percentage discrepancy of the average capacity of experimental and FEA results was only 3.86%. Therefore, due to less contribution of GFRP bars in the axial capacity of columns as compared with steel bars, it is recommended to use the GFRP bars in compression members where the involvement of reinforcement is less in axial loadcarrying capacity.(2)There is an impact of variation of viscosity parameter, dilation angle, and mesh size on the FEA results. The peak load of the control specimen increases up to 16% when the viscosity parameter increases from 0.0018 to 0.0068. Moreover, the peak load increases up to 13% when mesh size decreases from 60 mm to 15 mm. The effect of the dilation angle was only 4.75% when it increases from 30° to 45°. The effect of the element types on loaddeflection behavior was negligible. Therefore, the viscosity parameter and the mesh size appear to be critical for achieving the accurate results.(3)Even small eccentricities caused by the construction errors and the geometrical imperfections of construction materials in GFRPreinforced columns are of the great importance because they can cause a significant reduction in ultimate axial capacity of columns. In the presented FEA simulations, approximately a 39.74% reduction of the axial capacity of GFRP columns occurred for 25 mm eccentricity and 60.62% reduction occurred for 45 mm eccentricity when compared with an identical concentric column.(4)The FEA results obtained from ABAQUS in terms of loaddeflection curves were found to be consistent with the experimental results. The average discrepancies were 3.86% and 15.20% for steelreinforced columns and 3.78% and 18.54% for GFRPreinforced columns for loads and deflections, respectively. The material models used for numerical simulations produced slight overestimations for concentric columns. The premature failure of some eccentric columns occurred due to the opening of stirrups which caused the discrepancies. So, in future, it is endorsed to use the stirrups with lapped distance in ABAQUS simulations to avoid the premature failure of specimens. However, the FEA results show the capability of the selected numerical model for the prediction of loaddeformation behavior of steel and GFRPreinforced columns.(5)The numerical parametric study of one steelreinforced control specimen and one GFRPreinforced control specimen showed that the ultimate capacity of columns increases with the increase of compressive strength of concrete, with the increase of longitudinal reinforcement ratio and with the decrease of concrete cover. Furthermore, the squareshaped column was found to be the most efficient. The numerical parametric study results also confirmed the lower efficiency of GFRP bars in columns.(6)The cracking patterns were also studied in current research showing the crushing of concrete in columns. The cracking pattern can be visualized through tensile principal stresses and maximum positive principal plastic strains, but the latter gives a better representation of cracking patterns. A good agreement was achieved for FEA cracking patterns in comparison with experimental cracks. As an assessment tool, the importance of FEA software ABAQUS is that the parametric studies of structural members can be done which are not possible by experimental investigations.(7)The average percentage discrepancy of FEA results of steel RC concentric columns from empirical results was 8.45% and that of GFRP RC concentric columns was 2.44% using the design equation provided by MZ Afifi et al. Therefore, it is concluded that the presented FE model agreed well with experimental as well as theoretical results and can be utilized as a powerful and efficient numerical tool for the future studies on columns.
Data Availability
The data used to support the findings of this study are available from the corresponding author upon request.
Conflicts of Interest
The authors declare that they have no conflicts of interest.
References
 G. B. Maranan, A. C. Manalo, B. Benmokrane, W. Karunasena, and P. Mendis, “Behavior of concentrically loaded geopolymerconcrete circular columns reinforced longitudinally and transversely with GFRP bars,” Engineering Structures, vol. 117, pp. 422–436, 2016. View at: Publisher Site  Google Scholar
 A. De Luca, F. Matta, and A. Nanni, “Behavior of fullscale glass fiberreinforced polymer reinforced concrete columns under axial load,” ACI Structural Journal, vol. 107, no. 5, p. 589, 2010. View at: Publisher Site  Google Scholar
 H. Tobbi, A. S. Farghaly, and B. Benmokrane, “Behavior of concentrically loaded fiberreinforced polymer reinforced concrete columns with varying reinforcement types and ratios,” ACI Structural Journal, vol. 111, no. 2, 2014. View at: Publisher Site  Google Scholar
 H. M. Mohamed, M. Z. Afifi, and B. Benmokrane, “Performance evaluation of concrete columns reinforced longitudinally with FRP bars and confined with FRP hoops and spirals under axial load,” Journal of Bridge Engineering, vol. 19, no. 7, Article ID 04014020, 2014. View at: Publisher Site  Google Scholar
 W. Prachasaree, S. Piriyakootorn, A. Sangsrijun, and S. Limkatanyu, “Behavior and performance of GFRP reinforced concrete columns with various types of stirrups,” International Journal of Polymer Science, vol. 2015, Article ID 237231, 9 pages, 2015. View at: Publisher Site  Google Scholar
 S. Rizkalla, T. Hassan, and N. Hassan, “Design recommendations for the use of FRP for reinforcement and strengthening of concrete structures,” Progress in Structural Engineering and Materials, vol. 5, no. 1, pp. 16–28, 2003. View at: Publisher Site  Google Scholar
 B. Benmokrane, E. ElSalakawy, A. ElRagaby, and S. ElGamal, “Performance evaluation of innovative concrete bridge deck slabs reinforced with fibrereinforcedpolymer bars,” Canadian Journal of Civil Engineering, vol. 34, no. 3, pp. 298–310, 2007. View at: Publisher Site  Google Scholar
 L. C. Bank, Composites for Construction: Structural Design with FRP Materials, John Wiley & Sons, Hoboken, NJ, USA, 2006.
 T. T. Nguyen, T. M. Chan, and J. T. Mottram, “Influence of boundary conditions and geometric imperfections on lateraltorsional buckling resistance of a pultruded FRP Ibeam by FEA,” Composite Structures, vol. 100, pp. 233–242, 2013. View at: Publisher Site  Google Scholar
 W.r. Yang, X.j. He, and L. Dai, “Damage behaviour of concrete beams reinforced with GFRP bars,” Composite Structures, vol. 161, pp. 173–186, 2017. View at: Publisher Site  Google Scholar
 A. M. Amiri, A. Olfati, S. Najjar, P. Beiranvand, and M. H. Naseri Fard, “The effect of fly ash on flexural capacity concrete beams,” Advances in Science and Technology Research Journal, vol. 10, no. 30, pp. 89–95, 2016. View at: Publisher Site  Google Scholar
 M. A. Najafgholipour, S. M. Dehghan, A. Dooshabi, and A. Niroomandi, “Finite element analysis of reinforced concrete beamcolumn connections with governing joint shear failure mode,” Latin American Journal of Solids and Structures, vol. 14, no. 7, pp. 1200–1225, 2017. View at: Publisher Site  Google Scholar
 S. H. Alsayed, Y. A. AI·Salloum, T. H. Almusallam, and M. A. Amjad, Concrete Columns Reinforced by Glass Fiber Reinforced Polymer Rods, American Concrete Institute, Farmington Hills, MI, USA, 1999.
 F. Nunes, M. Correia, J. R. Correia, N. Silvestre, and A. Moreira, “Experimental and numerical study on the structural behavior of eccentrically loaded GFRP columns,” ThinWalled Structures, vol. 72, pp. 175–187, 2013. View at: Publisher Site  Google Scholar
 G. Turvey and Y. Zhang, “A computational and experimental analysis of the buckling, postbuckling and initial failure of pultruded GRP columns,” Computers & Structures, vol. 84, no. 2223, pp. 1527–1537, 2006. View at: Publisher Site  Google Scholar
 M. Elchalakani and G. Ma, “Tests of glass fibre reinforced polymer rectangular concrete columns subjected to concentric and eccentric axial loading,” Engineering Structures, vol. 151, pp. 93–104, 2017. View at: Publisher Site  Google Scholar
 A. Mirmiran, K. Zagers, and W. Yuan, “Nonlinear finite element modeling of concrete confined by fiber composites,” Finite Elements in Analysis and Design, vol. 35, no. 1, pp. 79–96, 2000. View at: Publisher Site  Google Scholar
 T. C. Rousakis, A. I. Karabinis, P. D. Kiousis, and R. Tepfers, “Analytical modelling of plastic behaviour of uniformly FRP confined concrete members,” Composites Part B: Engineering, vol. 39, no. 78, pp. 1104–1113, 2008. View at: Publisher Site  Google Scholar
 A. I. Karabinis, T. C. Rousakis, and G. E. Manolitsi, “3D finiteelement analysis of substandard RC columns strengthened by fiberreinforced polymer sheets,” Journal of Composites for Construction, vol. 12, no. 5, pp. 531–540, 2008. View at: Publisher Site  Google Scholar
 B. Piscesa, M. M. Attard, and A. K. Samani, “Threedimensional finite element analysis of circular reinforced concrete column confined with FRP using plasticity model,” Procedia Engineering, vol. 171, pp. 847–856, 2017. View at: Publisher Site  Google Scholar
 B. Alfarah, F. LópezAlmansa, and S. Oller, “New methodology for calculating damage variables evolution in Plastic Damage Model for RC structures,” Engineering Structures, vol. 132, pp. 70–86, 2017. View at: Publisher Site  Google Scholar
 O. Youssf, M. A. ElGawady, J. E. Mills, and X. Ma, “Finite element modelling and dilation of FRPconfined concrete columns,” Engineering Structures, vol. 79, pp. 70–85, 2014. View at: Publisher Site  Google Scholar
 W. X. M. Liu and Z. Chen, “Parameters calibration and verification of concrete damage plasticity model of Abaqus,” Industrial Construction, vol. 44, pp. 167–213, 2014. View at: Google Scholar
 Dassault Systems Simulia Corporation, ABAQUS Analysis User’s Manual 6.10EF, Dassault Systems Simulia Corporation, Providence, RI, USA, 2010.
 V. K. Papanikolaou and A. J. Kappos, “Confinementsensitive plasticity constitutive model for concrete in triaxial compression,” International Journal of Solids and Structures, vol. 44, no. 21, pp. 7021–7048, 2007. View at: Publisher Site  Google Scholar
 P. Kmiecik and M. Kamiński, “Modelling of reinforced concrete structures and composite structures with concrete strength degradation taken into consideration,” Archives of Civil and Mechanical Engineering, vol. 11, no. 3, pp. 623–636, 2011. View at: Publisher Site  Google Scholar
 S. Majewski, The Mechanics of Structural Concrete in Terms of ElastoPlasticity, Publishing House of Silesian University of Technology, Gliwice, Poland, 2003.
 C. E. De Normalisation, Eurocode 2: Design of Concrete Structures—Part 11: General Rules and Rules for Buildings, European Committee for Standardisation, Brussels, Belgium, 2004.
 P. Desayi and S. Krishnan, “Equation for the stressstrain curve of concrete,” ACI Journal Proceedings, vol. 61, no. 3, 1964. View at: Publisher Site  Google Scholar
 J. B. Mander, M. J. N. Priestley, and R. Park, “Theoretical stressstrain model for confined concrete,” Journal of Structural Engineering, vol. 114, no. 8, pp. 1804–1826, 1988. View at: Publisher Site  Google Scholar
 R. Nayal and H. A. Rasheed, “Tension stiffening model for concrete beams reinforced with steel and FRP bars,” Journal of Materials in Civil Engineering, vol. 18, no. 6, pp. 831–841, 2006. View at: Publisher Site  Google Scholar
 B. L. Wahalathantri, D. P. Thambiratnam, T. H. T. Chan, and S. Fawzia, “A material model for flexural crack simulation in reinforced concrete elements using ABAQUS,” in Proceedings of the First International Conference on Engineering, Designing and Developing the Built Environment for Sustainable Wellbeing, Queensland University of Technology, Brisbane, Australia, April 2011. View at: Google Scholar
 P. Wong, F. Vecchio, and H. Trommels, “VecTor2 and FormWorks user’s manual,” Department of Civil Engineering, University of Toronto, Toronto, Canada, 2002, Technical Report. View at: Google Scholar
 A. S. Genikomsou and M. A. Polak, “Finite element analysis of punching shear of concrete slabs using damaged plasticity model in ABAQUS,” Engineering Structures, vol. 98, pp. 38–48, 2015. View at: Publisher Site  Google Scholar
 M. Elchalakani, A. Karrech, M. Dong, M. S. Mohamed Ali, and B. Yang, “Experiments and finite element analysis of GFRP reinforced geopolymer concrete rectangular columns subjected to concentric and eccentric axial loading,” Structures, vol. 14, pp. 273–289, 2018. View at: Publisher Site  Google Scholar
 A. M. A. Ibrahim, M. F. M. Fahmy, and Z. Wu, “3D finite element modeling of bondcontrolled behavior of steel and basalt FRPreinforced concrete square bridge columns under lateral loading,” Composite Structures, vol. 143, pp. 33–52, 2016. View at: Publisher Site  Google Scholar
 D. I. Kachlakev and T. Miller, Finite Element Modeling of Reinforced Concrete Structures Strengthened with FRP Laminates, Oregon Department of Transportation Research Group & Federal Highway Administration, Washington, DC, USA, 2001.
 J. Lee and G. L. Fenves, “A plasticdamage concrete model for earthquake analysis of dams,” Earthquake Engineering & Structural Dynamics, vol. 27, no. 9, pp. 937–956, 1998. View at: Publisher Site  Google Scholar
 J. Lee and G. L. Fenves, “Plasticdamage model for cyclic loading of concrete structures,” Journal of Engineering Mechanics, vol. 124, no. 8, pp. 892–900, 1998. View at: Publisher Site  Google Scholar
 G. Z. Voyiadjis and Z. N. Taqieddin, “Elastic plastic and damage model for concrete materials: Part Itheoretical formulation,” International Journal of Structural Changes in Solids–Mechanics and Applications, vol. 1, no. 1, pp. 31–59, 2009. View at: Google Scholar
 J. Y. Wu, J. Li, and R. Faria, “An energy release ratebased plasticdamage model for concrete,” International Journal of Solids and Structures, vol. 43, no. 34, pp. 583–612, 2006. View at: Publisher Site  Google Scholar
 K. T. Nguyen, N. Ahn, T. A. Le, and K. Lee, “Theoretical and experimental study on mechanical properties and flexural strength of fly ashgeopolymer concrete,” Construction and Building Materials, vol. 106, pp. 65–77, 2016. View at: Publisher Site  Google Scholar
 N. F. Hany, E. G. Hantouche, and M. H. Harajli, “Finite element modeling of FRPconfined concrete using modified concrete damaged plasticity,” Engineering Structures, vol. 125, pp. 1–14, 2016. View at: Publisher Site  Google Scholar
 M. Z. Afifi, H. M. Mohamed, and B. Benmokrane, “Axial capacity of circular concrete columns reinforced with GFRP bars and spirals,” Journal of Composites for Construction, vol. 18, no. 1, Article ID 04013017, 2013. View at: Publisher Site  Google Scholar
 K. Kobayashi and T. Fujisaki, “32 compressive behavior of FRP reinforcement in nonprestressed concrete members,” in Proceedings of the Second International RILEM Symposium on NonMetallic (FRP) Reinforcement for Concrete Structures, CRC Press, Ghent, Belgium, August 1995. View at: Google Scholar
 H. Tobbi, A. S. Farghaly, and B. Benmokrane, “Concrete columns reinforced longitudinally and transversally with glass fiberreinforced polymer bars,” ACI Structural Journal, vol. 109, no. 4, 2012. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2019 Ali Raza et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.